The extraction of specific valuable minerals from their naturally occurring ores is variously termed "ore dressing," "mineral dressing," and "mineral beneficiation." For most metalliferous ores produced by mining operations, this extraction process is an important intermediatestep in the transformation of natural ore to pure metal. Although a few mined ores contain sufficient metal concentrations to require no beneficiation (e.g., some iron ores), most contain relatively small amounts of the valuable metal, from perhaps a few percent in the case ofbase metals to a few parts per million in the case ofpre cious metals. As Chapters 7, 9, and 10ofthis book have amply illustrated, the minerals containing valuable metals are commonly intergrown with eco nomically unimportant (gangue) minerals on a microscopic scale. It is important to note that the grain size of the ore and associated gangue minerals can also have a dramatic, and sometimes even limiting, effect on ore beneficiation. Figure 11.1 illustrates two rich base-metal ores, only one of which (11.1b) has been profitably extracted and processed. The McArthur River Deposit (Figure I 1.1 a) is large (>200 million tons) and rich (>9% Zn), but it contains much ore that is so fine grained that conventional processing cannot effectively separate the ore and gangue minerals. Consequently, the deposit remains unmined until some other technology is available that would make processing profitable. In contrast, the Ruttan Mine sample (Fig. 11.1 b), which has undergone metamorphism, is relativelycoarsegrained and is easily and economically separated into high-quality concentrates. Most mineral beneficiation operations involve two principal stages. The first of these is reduction in size of the particles of mined ore (which may
326 INTRODUCT ION 327
(bi FIGURE 11.1 Differences in gra in size reflect the origin and history ofa deposit an d may affect the comminution and recovery of an ore. (a) Very fine-grained spha lerite and pyrite that are difficult to separate and recover prevent ed efficient processingofthe rich (9%Zn) and large (> 220 million ton s) but unmetam orphosed McArthur River De posit, Australia.(b) Metam orph ism recrystallized and coa rsened the pyrite, spha lerite, and galena in the ores of the Rutt an Min e, Ca nada, and permitted easy sepa ration and recovery (width of field = 1,200 11m, the same in bo th photographs). initia lly be bloc ks up to several meters in dia mete r) to a size th at is as close as possible to th at ofthe individu al metal-bearing mineral particles .This process ofcomminution achieves the liberation of valuable minerals from th e ga ngue and, in the case ofcomplex ores,libe rat ion ofdifferent valuab le mineral s from one anot her. Since the size redu ction required to achie ve liberation is co m mo nly down to a few hundreds ofmicron s or less in diameter, exte nsive crush ing followe d by grinding (orm illing )ofthe ores is req ui red .Th e second stage in beneficiation is th at of m ineral separation, in whic h the valuable minerals are rem oved as a concentrate tc t concentratesi and th e remaining.cornmonly value- 328 APPLICATIONS OF ORE MICROSCOPY IN MINERAL TECHNOLOGY less materials (the tailings) are discarded. This separation is usually achieved by exploiting differences in the physical, chemical,or surface properties ofore and gangue minerals. For example, the fact that many metalliferous ores are more dense than associated gangue minerals can be exploited by using heavy media for separation or other methods of gravity concentration, such as mineral jigs or shaking tables. The fact that certain ore minerals are strongly attracted by magnetic fields (e.g.,magnetite, monoclinic pyrrhotite) or exhibit metallic or semiconducting electrical properties can be exploited in certain magnetic and electrical methods of separation. However, the most widely employed method ofseparation isfrothflotation, in which the surface chemis try offine ore particles suspended in an aqueous solution is modified by addi tion ofconditioning and activating reagents to be selectively attracted to fine air bubbles that are passed through this suspension or pulp. These air bubbles, with the associated mineral particles, are trapped in a froth that forms on the surface of the pulp and can be skimmed off to effect the separation. The technical details ofthe various comminution and separation methods are beyond the scope ofthis book and can be obtained from works by Pryor (1965), Gaudin (1957), and Willis (1992). However, in the study ofthe mined ores and the products ofvarious stages of the comminution and separation processes, ore microscopy has a very important industrial application. It facilitates the identification ofthe valuable minerals and of minerals that may prove troublesome during beneficiation or during later stages ofextraction. It also provides information on the sizes of particles, the nature of their inter growth, and the nature of the boundaries (Tocking") between them. The efficiency of comminution and separation techniques can be monitored at any stage by the examination ofmounted and polished products underthe ore microscope. Thus, from the initial assessment of the commercial exploit ability ofa prospective ore through the planningofa processing plant, the set ting up of a pilot plant, and the first efficient operation of the full-scale beneficiation scheme, a vital role is played by the ore microscopist. Certain ores, rather than undergo the complete processes ofcomminution and physical particle separation described previously/may have the valuable metals removed from them by chemical dissolution. For example, gold maybe dissolved by cyanide solutions, orcopperin the form ofcoppersulfides may be dissolved (leached) by acid solutions. When crushing and grindingofthe ores is required to expose the minerals to the action of the solutions, ore micro scopy is again important in planning and monitoring efficient cyanidation or acid leaching. The technologies of such processes lie more in the general field of metallurgy than that of mineral beneficiation, although the term mineral technology can be taken to embrace all of them. In this chapter, the appli cations ofore microscopy in mineral technology will be considered.Although the products ofthe roasting and smelting ofores that follow beneficiation are sometimes substances with no natural (mineral) equivalents, the techniques ofore microscopy remain applicable. MINERAL IDENTIFICATION IN MINERAL BENEFICIATION 329
Further information on the subject discussed in this chapter may be found in works by Schwartz (1938), Edwards (1954), Gaudin (1957), Amstutz (1961), Rehwald (1966), Ramdohr (1969), and Hagni (1978). The range of textural information that is required in mineral beneficiation and obtainable pri marily from ore microscopy is summarized in Table 11.1.
11.2 MINERAL IDENTIFICATION IN MINERAL BENEFICIATION
The techniques described in earlierchapters ofthis book(Chapters 3,5,and 6) can all, of course, be applied in the identification of opaque minerals in both untreated ores and products of various stages ofcomminution or separation. The first concern in the untreated ore is identification ofphase(s) thatcarrythe valuable metal(s), since the initial information available is commonly only a bulk chemical analysis of the ore. This analysis provides no information on the mineral phases present nor on their sizes and textural relations; it is pos sible for different mineral associations to yield very similar bulk analyses. For example, nearly all zinc ores contain sphalerite as the only or principal zinc bearing phase. In rare, but sometimes important deposits (e.g., Sterling Hill, New Jersey), the zinc is held as zincite (ZnO) or willemite (Zn2Si04), or both. Another possible significant zinc phase is gahnite (ZnAl204). Each of these zinc minerals has the potential to form ores, but their different physical pro perties make their processing and the extraction of zinc very different. Hence, the determination of the type of metal-bearing phase(s) is critical. As outlined by Schwartz (1938) and by Ramdohr (1969), the precise iden tification and characterization of the ore minerals can save a great deal of work in the establishment ofan efficient beneficiation system. Examination of the untreated ore will enable the assessment of the feasibility ofusing den sity, magnetic, or electrical methods of separation, since such properties are wellcharacterized for most minerals. However, fine intergrowths of dense ore minerals with gangue phases can result in ranges in specific gravity and loss of valuable metals or dilution of concentrate.' Similar problems can arise from fine intergrowths of"magnetic" and "nonmagnetic" phases (e.g., removal of ferrimagnetic magnetite and pyrrhotite from the nickel-bearing pentlandite in the Sudbury ores may result in nickel losses due to fine pentlandite flames in the pyrrhotite). The flotation properties of most ore minerals have also been extensively studied, so identification is an important first step in the applica tion of this separation method. However, flotation behavior can be very ad versely affected by oxide coatings or by tarnishing of ore mineral grains; such coatings may be detected under the microscope and either removed by acids prior to flotation or subjected to flotation using different reagents. Inefficient
1When certain methods of separation are used. such material may appear in a third. intermediate fraction that is between concentrate and tailings in composition and is termed the "middlings." TABLE 11.1 Information Available from Mineralogic Studies Compositional or Mineralogic Data Subdivided into Metallic ore minerals (and/o r) Nonmetallic ore min erals Non ore metallic (pyri te. etc.) Gangue min erals With special reference to (selection of exa mples) Specific gravity Solubility Rad ioactivity Magnetic properties Cleavability (sliming properties. sheeting and coa ting properties. such as sericite. clays. talc. covellite, etc.) New ph ases in artificial products (slags. matt es. speisses, sinters, etc.) State of oxida tion Obj ectionable minerals (minerals with P. S. As in certain iron ores or Bi in lead ores. etc.) Chemica l composition of min erals (othe r elements contained in solid solution. like Fe in sphalerite. Ag in tetrahedrite, etc.) On the basis ofthe aforementioned information. the best method of con cent rating ca n be chosen. Co mpos itiona l changes to be expec ted in the wall rock. in adjacent zones (oxidation.enrichment. leaching.etc.),or at depth. which will bear on the milling operations. as mining pro ceeds
Geometric Data (Texturesand Structures) Of Metallic ore minerals (and/o r) Nonmetallic ore min erals Non ore metallic minerals G an gue minerals With special infor mation on Locking types (includ ing such data as tarnish. coa ting, veining. etc.), porosity. pitting, etc. Quantitative data Amounts of metallic ore min erals (and/o r) Amounts of nonmetallic ore min erals (an d/or) Amounts of non ore metallic min erals (and/o r) Amo unts of gangue minerals With quantitative information on the qualit ative and geometric properties listed ab ove. for example. Relative grain size or particl e size Relative size of locking Relative amou nts of lockin g (as a whole) Relati ve proport ion s of individu al minerals in the locked particles (middlings) Che mical analyses of sa mples (tailings. ores. concentrates. etc.), estimated or computed on the bas is of the particl e cou nting data
330 MINERAL IDENTIFICATION IN MINERAL BENEFICIATION 331 separation by flotation also occ urs when the particles co nsist ofgrains of more than one mineral phase th at are "locked" (bo und in so me manner) togeth er: the result is either loss ofo re mineral or co nta minatio n by the attac hed grains (Figure 11.2). Special problem s may also arise with ores that co nta in co mplex minerals (e.g.. minerals ofthe tetrahedrite gro up.altho ugh dominantly co ppe r sulfosalts, may co nta in high contents of zin c. mercury. or silver that will appear in the co nce ntrate). As well as assessme nt of the probl em s of mineral sepa ration following mineral identification. the efficiency of separation ca n be monitored by examination of products at the various stages of beneficia tion. In this regard. it is impo rta nt tha t tailings as well as co nce ntrates be thoroughly studied. Iden tificat ion and ch aracteri zat ion of the ore minerals is also important for subs equent metallurgical proc essing; for example. ti tanium is more difficult to ext rac t from ilmenite than fro m rut ile. The identification and cha rac terization of the ga ngue mi nerals, which may include worthless opa que phases. is also very impo rta nt. Th ese materials may have economic po ten tial, and their be havior during o re processing mu st be ass essed. Particul arl y important is the identification (a nd subseq uent re moval, in some cases) of impurities th at may adversely affect the efficiency of later co nce nt ratio n o r refining processes o r may lower the qua lity ofthe final product. An example of th e former is the presence of iron sulfides. stibnite. or coppe r sulfides in gold ores th at are to be treated by dissolution in cya nide solution: suc h materi als also react with th e cya nide solution. resulting in both its co nsumptio n and contamination.An exa mple ofthe latter is the presen ce of ph osphorus-b earing minerals in iron ores that reduce ore qu ali ty below tha t required for steel making. Probl em s ca n also arise from the presen ce of fine-l ayer silicates such as kaolin. talc . o r sericite wh en flotation is used for o re co nce ntra tion. Th ese minerals also tend to float and thus reduce the grade o f the co nce ntra te. Even the presen ce ofin ert gangue phases suc h as qu artz may be important in assessing efficient co m minution. Wh en such hard materials
FIG URE 11.2 Locked and unlocked num er al grains.A locked grain ofsphalerite and pyrr hotite coexis ting in a mill product with un locked grains of pyrite and pyrrhotite. Du cktown. Tennessee (width of field = 600 urn).
ORE TEXTURES IN MINERAL BENEFICIATION 333
The question of the sizes and size distributions of ore (and gangue) particles is closely linked to the important role of studies of ore textures in relation to beneficiation problems, which will now be discussed.
11.3 ORE TEXTURES IN MINERAL BENEFICIATION
Since the first stage in the beneficiation of ores in orderto liberate the particles of valuable minerals from each other and from the gangue is comminution, knowledge of the sizes and intergrowth relationships of ore mineral grains is of great importance. Only through careful examination ofthe ores in polished section can the optimum grain size for effective liberation be determined. Insufficient grinding may result in loss of valuable minerals in the tailings; overgrinding wastes energy and may produce slimes that are difficult to treat later in the processing stage. The efficiency ofthe grinding methods employed at the pilot stage must also be monitored by the examination ofpolished grain mounts of their products. The great variety of intergrowths that may occur between ore and gangue minerals and between different ore minerals that may eventually require separation has been well illustrated already (see Chapters 7, 9, and 10). As we consider the problems ofliberation of the ore minerals, it is useful to outline a fairly simple classification based on the geometry of the intergrowths and locking textures,without anygenetic implications. Such a classification oftex tures has been suggested by Amstutz (1961).This classification forms the basis of Figure 11.3, which also incorporates some information on the liberation characteristics ofthe ore types illustrated. As well as the type and scale of the intergrowths, the nature of the boun daries between intergrown particles is important. This will show whether or not the rupturing oflarger particles during grinding is likely to occur at grain boundaries. For similar reasons, information regarding fractures and fissures in the ore minerals, as well as the porosity ofthe material, is important data that is derived from examination under the microscope. In addition to the influence that such textural features have on the comminution process, they have importance in the flotation and leaching methods ofore treatment. The extent to which liberation has been achieved at each stage in grinding can, of course, be assessed by quantitative determination under the ore mic roscope. This may be seen in the photomicrographs ofground ores in Figure 11.4. Even if the desired ore minerals are more or less randomly distributed in an ore, their distribution into different size fractions during comminution may be controlled by their textures . Table 11.2 presents quantitative micro scopic data showing the distribution of ore and gangue minerals as functions of size fractions during grinding of the massive pyrite and pyrrhotite ores of the Ducktown,Tennessee, deposits.The data demonstrate that the valued ore minerals-chalcopyrite and sphalerite-are strongly concentrated in the finest fractions, whereas the pyrite is dominant in the coarse fraction.The cause lies in the initial ore texture, where chalcopyrite and sphalerite occur as small grains and film along the margins ofthe coarse pyrite crystals in a pyrrhotite Texture and Liberation Properties in Nature of Relatively Large Particles, Interlocking Diagram Examples of Ores
Equigranular. Fairly easy liberation . Com Straight, rectilin mon occurrence especially in ear, cuspate mar orthomagmatic and highly gins. Simple metamorphosed and recrystal locking. lized ores. Also in ores show ing successive depositional sequence.
Mutually curving Fairly easy liberation. Com boundaries with mon occurrence in simulta negligible inter neously crystallized ores where penetration. Sim interfacial free energies are ple locking. similar.
Mottled, spotty, Fairly easy liberation. Com careous, with par mon occurrence in ores where tial penetration. interreplacement processes Relatively simple have been active. locking.
Graphic, myrme Complete liberation difficult or kitic, visceral impossible. Not common as a locking. Deep mi major texture in ores. Pro cropenetration. duced by exsolution and re placement . Examples: galena/sphalerite and chalco cite/bomite.
FIGURE 11.3 Geometric classification of ore mineral textures and their liberation characteristics.
334 Texture and Liberation Properties in Nature of Relatively Large Particles, Interlocking Diagram Examples of Ores
Disseminated, Complete liberation difficult or droplike, emul impossible; chemical treatment sion, eutectoidal often required. Common oc locking. Finely currence by exsolution (left) dispersed phases. Au/arsenopyrite chalcopyrite/ sphalerite; by replacement (right) pyrite/sphalerite. Intergranular rim; Liberation may be difficult if coating mantled, free grain is continously envel enveloped, atoll oped by layer. Not uncommon ; like locking. often formed by replacement reaction. Examples: hematite film on gold; chalcocite or co vellite on pyrite, galena, or sphalerite. Concentric, spher Liberation fairly difficult or ulitic, scalloped, difficult; common occurrence colloform-Iayered in Fe, Mn, and Al ores. Also locking. U (pitchblende) intergrained with sulfide. Usually associated with colloidal precipitation.
Planar, lamellar, Liberation fairly easy to vari sandwich-type able. Produced by exsolution locking. Lamellae (examples: cubanite/chalcopy may vary in size. rite, ilmenite/magnetite). Also by replacement. Examples: magnetite and hematite.
Reticulate (net Liberation variable to difficult. like) boxwork. Common occurrence by re Finely interpene placement. Examples: bornite/ trating locking. chalcopyrite, anglesite/covelli te/galena. Also by exsolution. Examples: hematite/ilmenite/ magnetite.
FIGURE 11.3 (Continued)
335 FIGU RE 11.4 Photomicrographs of grain mounts of ground ores. (a) Ground ore prior to concentration (width offield = 520 11m). (b) Lead concentrate from Viburnum Trend. southeast Missouri; dominantly galena fragments with minor sphalerite (darker gray) (width of field = 520 11m).
336 EXAMPLES OF APPLICATIONS OF ORE MICROSCOPY IN MINERAL BENEFICIAT ION 337
TABLE 11.2 Microscopic Determination of Ore and Gangue Minerals from Mas sive Metal-bearing Sulfide Ore at Ducktown, Tennessee, as Functions of Size Fraction During Grinding
Min erals" (in %) Mesh Mi cron s Size (Approx.) Po Py C py Mt Sp h Gangue + 35 > 420 32 61 0.9 1.0 0.0 4.4 35-48 420-290 47 44 1.6 0.9 0.2 6.0 48-65 290-200 49 36 2.6 1.0 0.2 10.0 65- 100 200- 130 50 28 3.3 2.1 0.5 16.0 100-150 130-95 50 24 5.9 2.9 0.7 16.6 150-200 95-75 49 23 5.0 3.9 1.0 18.4 200-250 75-55 56 21 4.6 4.8 1.0 12.8 Source: C ra ig.J. R..Yoon. R. H.. Haral ick. R. M..C ho i. W. Z.. and Pong.T. C. ( 1984).Mineralogical Variations During Comminution ofComplex Sulfide Ores in Process Mineralogy III. W. Petr uk.ed..Soc. ofMining Engineers. New York . pp . 51-63. a po = pyrrh ot ite: py = pyrite: cp y = ch alcop yrite: mt = magnetite: sph = sphalerite. matri x. During grinding, the ores fracture along th e weakest zo nes, that is, through the cha lcopyrite a nd spha lerite, yielding numerous sma ll frag ments of these minerals and leaving th e harder pyrite crystals in large grains or fragment s. Detailed examination of each size fraction of an ore during com munication can reveal information on the conce ntration of ph ases during grinding as well as determine the degree to which the grains are liberated from othe r minerals.
11.4 EXAMPLES OF APPLICATIONS OF ORE MICROSCOPY IN MINERAL BENEFICIATION
A number ofcontrasting exa mples can be used to illustrate thi s applica tion of ore micro scopy.
11.4.1 Gold Ores Economi c occur rences of gold gene rally consist of very sma ll amo unts of dis persed native gold or gold-silver alloys. Even in the well-kn own ores of th e Witwatersrand in South Africa, the average conce ntration of gold is only about 16 ppm (0.5 troy oz/ton). The ores containing native gold may contai n large amounts of qu art z and minor (uneconomic) sulfides; little qu art z but large amounts ofvalueless sulfides (pyrite, pyrrhotite, arseno pyrite); or valu able ba se-metal sulfides of antimon y, arsenic, copper, lead. or zinc. Although some coa rser gold particles may be sepa rated from gangue by utili zin g th e high den sity of gold (cf. the "pa nning" of ea rly prospectors), mu ch gold is 338 APPLICATIONS OF ORE MICROSC OPY IN MIN ERAL TECHNOLOGY
removed from ore by dissolution in a cyanide solut ion (cyanidation) or in mer cury amalgam (now rarel y used and illegal in many places). For density sepa ration. the gold particles mu st be liberated from gangue; for cyanidation or a malga ma tion. the gold mu st be sufficientlyexposed to permit attack by the cya nide solution (or mercury). Th is is shown by two of the examples ofgold ores illustrated in Figures I L5a and I L5b. In the first case, gold occurs along grain boundaries and fractures. and. in the second. as minute particles withi n the sulfide. An equivalent amount of gri nding will produce a mu ch greater "effective liberation " ofgold in the first ore because ofthe ten den cy to break along fractures and boundaries. This ore ca n be subjected to cya nida tion after (or during) grinding. whereas the seco nd ore may need roasting to release the gold before it can be successfully cya nided. Man y ores will. ofcour se, contain a certain amo unt of both types of intergrowth: the relative amo unts and size ran ges ca n then be determined by microscopic exa mina tion. Ifgold particles occ ur largely as inclusion s in a particularphase (e.g.. pyrite), it may be possibl e to co nce ntra te thi s ph ase by flotation and subject only this to fine grinding or roas ting in orde r to lib erate the gold. When the cyanidation process is to be emp loyed in gold extraction. it is par ticul a rly important that microscopic studies be made to determi ne the pres ence ofdelete riou s mi nerals.Th e dissolution process depends on an adequate supply of oxygen; pyrrhotite, marcasite, and some pyrites consume oxyge n. thu s inhibiting the process. Other minerals. notab ly stibnite, copper sulfides. and so me a rsenopyrites a nd pyrite s may dis solve in the cyanide solution. resulting in excessive consumption ofcyanide and even reprecipitation ofthe gold in extreme cases. In cases in which the concentration of deleterious
..' ;": oJ .' If: ."".: . .. - , ,"-
.-- ~- ) I . ", f -. r - -: .. . '- " ... .:» (a ) ..,. .: ~ I FIGURE 11.5 Examples ofgold ores.(a) Gold occurring along grain boundaries and fractures in pyrite. Witwatersrand. South Africa (widt h of field = 2.000 urn). (b) Gold occurring within chalcopyrite. Witwatersran d. South Africa (width of field = 210 urn). (c) Gold grain coated with magnetite and goethite . Alaska (width of field = 2.000 urn).
339 340 APPLICATIONS OF ORE MICROSCOPY IN MINERAL TECHNOLOGY minerals is such that it seriously affects the efficiency of the process, it may be necessary to remove the minerals by flotation prior to cyanidation. As with cyanidation, certain minerals can adversely affect amalgamation (e.g., stib nite, enargite, realgar, tetrahedrite, pyrrhotite, arsenopyrite, and pyrite react with amalgam) and may have to be removed. Otherproblems in the processing ofgold ores may result from the presence of a coating on the surface of the gold particles (commonly ofiron oxide, as shown in Figure 11.5c). This can result in losses of gold during separation (especially if a magnetic process is employed to remove oxide impurities that may then carry gold with them) and can prevent dissolution of the gold unless it is removed by grinding. Other coatings that inhibit dissolution may form during processing. With an ore as valuable as gold, an important aspect of microscopic studies for efficient extraction is the examination oftailings. If losses are occurring in the tailings, the reasons for such losses can then be determined.
11.4.2 Copper Ores Copper is obtained largely from sulfide ores, and chalcopyrite is the single most important copper ore.mineral. The chemistry and metallurgy ofchalco pyrite have been reviewed by Habashi (1978). Other copper-iron (bornite, cubanite, talnakhite, mooihoekite) and copper(covellite, chalcocite, digenite, djurleite) sulfides are often associated with chalcopyrite and may be locally important. The coppercontent ofeach of these phases is different, and a care ful quantitative determination of the mineralogy is an important step in the assessment of are grade. Many of these phases (particularly bornite, chalco cite, and covellite) may result from the alteration of chalcopyrite in processes ofsecondary enrichment (see Figure 7.11). Examples of majorcopperdeposits are the porphyrycoppers (see Section 9.5),large deposits that are often mined at average copper concentrations ofless than 0.5%. Such deposits contain large amounts of pyrite as well as chalcopyrite; some copper may occuras sulfosalts (tetrahedrite, enargite), and silver and gold may also occur in small but economically important quantities. Quartz, feldspars, biotite, chlorite, seri cite, anhydrite, clay minerals, and other layer silicates are the dominant gangue minerals. ' As Gaudin (1957) has pointed out, the sulfide copper ores are particularly well suited to flotation recovery methods. When the are is largely chalcopyrite and pyrite, liberation of chalcopyrite can usually be achieved by normal grinding methods. Flotation can then be carried out to selectivelyconcentrate the chalcopyrite. The preparation of a copper concentrate may be more dif ficult if chalcopyrite, pyrite, and other copper sulfides are intimately inter grown.Anotherproblem may arise in recovering the gold or silver,which may well follow pyrite into a "tailings fraction." Solutions to all of these problems require careful study of mined ores and mill products by are microscopy. EXAMPLES OF APPLICATIONS OF ORE MICROSCOPY IN MINERAL BENEFICIATION 341
When the ores have been partly oxidized, some ofthe copper may be pres ent as easily soluble oxides , basic sulfates, or carbonates from which copper can be easily extracted by acid leaching. Such methods are being more widely employed also as a method of extraction of copper from sulfides in dump leaching ofvery low-grade ores (Fletcher, 1970). Here again, microscopic study of textures to estimate the efficiency of the leaching process is important. Anothermajorsource ofcopperis the volcanogenic massive sulfide deposit (Section 10.9). The chalcopyrite in these ores occurs as anhedral interstitial grains and to a variable butsignificant extent as very small « 5 11m) blebs and veinlets within sphalerite ("chalcopyrite disease," Figure 7.18).This finely dis persed chalcopyrite can create separation problems and may result in ap preciable copper reporting in the zinc concentrate. It may also be desirable to remove, during beneficiation, certain phases that cause problems during smelting (e.g.,arsenopyrite in order to reduce arsenic emissions). Such prob lems are readily anticipated if detailed ore microscopic work has first been undertaken.
11.4.3 Chromium Ores The only significant ore mineral ofchromium is chromite (ideal composition, FeCr204), which occurs in ultramafic and mafic igneous rocks (see Section 9.2).Although chromite often occurs in a silicate matrix (see Figures 9.1 and 9.2) as single-phase euhedral-subhedral grains that can be readily separated by grinding and gravity concentration, deficiencies in the grade ofa concen trate may result from intimate intergrowths with gangue minerals orvariation in chromitecomposition.The former is often a result ofsevere fracturing ofthe chromite and infilling ofthe fractures with serpentine; the latter results from the substitution ofFe!" and Al3+ for Cr3+ in the chromite, the composition of which may even vary within a single grain, producing a zonal distribution of chromium concentration. Variations in magnetic properties ofchromites as a function of iron content may permit selective magnetic concentration of chromium-rich fractions in some cases. The efficient gravity concentration of low-grade chromite ore from Cyprus described by Mousoulos and Papa dopoulos (1976) involved a combination of heavy media, jigs, and shaking tables.
11.4.4 Iron-Titanium Oxide Ores Some iron-titaniumoxide ores present particularmilling problems because of the intimate association of the mineral phases. Figure 11.6 illustrates two extreme examples ofores: in Figure 11.6a, the separation is readily achieved; in Figure 11.6b, the separation is difficult to achieve. In the former case, ilmenite and magnetite coexist in a coarse equigranular aggregate and can FIGURE 11.6 Examples of iron-titanium oxide ores. (a) Co arse magnetite grain (dark gra y. pitted) flanked by coa rse ilm enite grains. Storgangen, Norway (width of field = 2.000 11m). (b) Fine lam ellae of hematite with in ilmenite. Blasfjell, Norway (width of field = 520 11m).
342 THE STUDY OF SMELTER AND INCINERATOR PRODUCTS 343 readily be separated magnetically after grinding. In the latter case , however, the intimate intergrowth ofilmenite with hematite, down to a submicroscopic scale, makes a clean mechanical separation of the phases impossible.
11.4.5 Manganese Nodules The manganese nodules ofthe deep ocean floors are an important potential source of not only manganese but also ofother base metals; nodule deposits being considered for mining assay as high as 2.3% Cu, 1.9% Ni, 0.2% Co, and 36%Mn (dry weight) (Fuerstenau and Han, 1977).Study ofthe nature and dis tribution of the phases containing these valuable metals in the nodules is an important step toward their economic exploitation. Although their detailed mineralogy is complex, the predominant minerals in the nodules are manga nese (IV) oxides related to the terrestrial minerals todorokite, birnessite, and cS Mn02; also present is crystallographically poorly ordered goethite ("incipient goethite") (Burns and Burns, 1977; 1979). The nickel, copper, and cobalt are taken up by todorokite in postdepositional processes. The textural relation ships between mineral phases in a nodule are shown in Figures ll.7a and ll.7b. Brooke and Prosser (1969) examined the mineralogy and porosity ofsev eral such nodules and investigated the problem ofselective extraction ofcop per and nickel. Tests showed that selective leachingofcopper and nickel using dilute sulfuric acid is a possible method ofextraction. A whole range of pos sible extraction methods (acid leaching, ammonia leaching, smelting, chlor ination, and segregation roasting) have also been reviewed by Fuerstenau and Han (1977).
11.5 THE STUDY OF MATTES, SLAGS, ASHES, SINTER, AND OTHER SMELTER AND INCINERATOR PRODUCTS
The compositions and textural relationships ofthe products ofsintering and smelting (mattes, slags, etc.) can be studied by using the techniques outlined in Chapters 1-6. Although these are not minerals, many do closely resemble ore minerals in composition and optical properties and sometimes in texture. Their history of crystallization may also be followed using textural inter pretations similar to those outlined for ores . Slags (Figure 11.8),the waste products ofsmelting, are intended to remove impurities from the desired metals. Ideally, all ofthe metal remains in a melt, whereas all impurities segregate into the slag. In reality, the separation is never perfect, and studies ofthe slags and matterare used to reveal the quantities and nature of phases eitherlost or serving as contaminants. The loss of some iron duringsmelting(Figure 11.8b) is generallyoflittle economic consequence, but the loss of copper(Figure 11.8d)is of concern, and the loss ofelectrum (Figure 11.8a) in the smelting of gold and silver ores can be very serious. FIGURE 11.7 Textural relationships between mineral phases in manganese nodules sectioned in different orientations. (a) Blake Plateau. Atlantic Ocean (width offield = 2.000 11m). (b) Pacific Ocean (width of field = 520 11m).
344 THE STUDY OF SMELTER AND INCINERATOR PRODUCTS 345
Th e mining and smelting ofiron is much larger and widespread than th at of any other metal. The study by Bast a, EI Sharkowi, and Salem (1969) pro vides an exa mple of iron slags.They studied the mineralogyoff1uxed sinters of fines from the Aswan iron are. Th ese oolitic ores are mainly hem atite, with some goethite, quartz, carbo na te, and chlorite; some minor sulfur, ph osph orus, a nd manganese are also present. Sintering was at ~ I,200°C, with limestone, pyrite cinde rs, and coke as a fuel. Studies of such sinters show iron, iron oxides
FIGURE 11.8 (a) Sph eres of electrum occurring in slag from the smelting of gold silver ores. Such entrapment requires remelting ofthe slag to recover all of the precious metals, Morning Star Mine, California (width offield = 1,200 11m ). (b) Dendritic crys tals of magnetite in a matrix ofglass; sinter from Aswan iron ore (width offield = 200 11m ). (Reproduced from E. Z. Basta et al.,Trans. I.M.M. 78, C3, 1969;used with permi s sion.) (c) Copper-nickel matte with small euhedral crystals of Fe, Ni disulfide in a ma trix of'Cu jS (dark gray) and NiS (light gray). A large subhedral grain of metallic nickel is visible in the upp er-left-hand corner (width of field = 2,000 11m). (d ) Dendritic crys tals of magnetite with interstitial pyrrhotite and chalcopyrite in ancient slags produced by the Rom an s as they worked the copper ores on Cypru s (width of field = 1,200 11 m) . 346 APPLICATIONS OF ORE MICROSCOPY IN MINERAL TECHN OLOGY
ldl FIGURE 11.8 (Continued)
(magnetite, hem atit e, wustite), and calcium ferrites as sp he rules, dendrites, a nd crystals in a matrix ofsilicates- both crystalline (gehlenite, olivine, wol lastonite) and glassy (Figure 11.8b). Minor sulfides may also be present (pyr rhotite, cha lcopyrite). The effect of varying the amounts ofl imesto ne ad de d is related to min eralogical vari ations that are , in turn, related to suc h properties as strength and reducibility of th e sinters. The reduction ofilmenite has been studied byJones (1974).At temperatures less than LOOO °C, natu ral ilme nites are reduced by carbon mon oxide to metallic iron and redu ced rutiles (Til/02l/- I ,!1 ;;;. 4), but minor magnesium or man gan ese prevent the reaction from going to completion. Th ese problems are lessen ed at higher temperatures, and at 1,200°C the products ofreduction are metalli c iron and anosovite (Fe3-xTixOs) solid solution. These reaction produ cts were characterized at va rious stages ofreduction by ore mic roscop y (a nd electron probe micro an alysis). Th e mattes produced in coppe r smelters vary conside ra bly in co mpos ition but include many ofthe ph ases familiar from mineralogical studies in the Cu Fe-S and Cu-Ni-S systems. Figure 11.8c illustrate s the nature of a copper- THE STUDY OF SMELTER AND INCINERATOR PRODUCTS 347 nickel matte containing 40% Cu and 40% Ni. Th e matte contains an ea rly crystallized iron-nickel alloy ph ase, dispersed sma ll grains of an Fe-Ni di sulfide and a matrixofNiS (millerite), and a cop persulfide solid solution.This last phase has exsolved on cooling to give a basket weave texture oftwo copper sulfide ph ases. Figure l 1.8d is a Rom an-period coppe r mining slag from Cy pru s; it reveals the loss ofcopper and ch alcopyrite associated with magn etite and pyrrhotite in the slag. The combustion ofcoal , oil, and even municip al solid waste conce ntrates metals and gene rates ashes and slags th at contain mineral-l ike phases. Coals generally contain significant qu antities ofclays and qu artz in addition to trace to minor amounts of metals and metal-bearing ph ases (especially pyrite). During combustion, the metal s and other nonflammabl e materials becom e concentrated by factors of about 10 tim es, with the resultant formation of spinel-type oxid es, several silica te ph ases, a nd occasional iron sulfides in a glassy silicate matrix. Th e distill ation ofpetroleum to leave a solid coke-like ph ase, and th e subse quent combustion of that material, result s in a much greater degree ofconce n tration (approximately 1,000times) of metals a nd sulfur, but with mu ch less silica. The resulting slag may contain a complex variety of iron, nickel, and vana dium sulfides and oxides, as well as mu ch free metal (usually as iron nickel alloys), as shown in Figure 11.9. Microscopic ana lysis has revea led much abo ut the ph ases present and their potential for reuse or disposal (C raig, Najjar, and Robin, 1990; Groen, 1992).
(a ) FIGURE 11.9 Scanning electron microscope images of petroleum coke slags. (a ) Atoll-like structure ofnative iron and some cruciform spinel crystals in a fine matrix of inte rgrown FeS and FeO in slag produced during production of synthesis gas from petroleum coke (width offield = 100urn). (b) Equ ant and skeletal crystals of iron- and nicke l-rich aluminate spinels in a matrix of glass from a petroleum coke gasifier. The coarser crystal s were probablystable at the temperatureofthe gasifier, wherea s the very fine crystals formed during rapid cooling of the glass (width of field = 360 urn). 348 APPLICATIONS OF ORE MICROSCOPY IN MIN ERAL TECHNOLOGY
(a ) FIG URE 11.9 (Continued's
T he inci neration ofmunicipal solid waste is bei ng undertaken mo re wide ly to generate heat and to effect volume redu ction .As one migh t expect. the ashes and slags produced are rich in silica tes and glasses bu t co nta in a wide variety ofmetall ic mineral-like oxide ph ases (Brock, 1993; Kirby a nd Rim stidt, 1993). Mu ch more study is needed to characterize all of the phases present and to identify potential uses or problem s related to their ultim ate dispo sal.
11.6 CONCLUDING REMARKS
This very brief outline of th e applicatio ns of ore microscop y in mineral technology serves only to illu st rate the great importance of this area of ap plication. Th e inc reasing world de ma nd for metals necessitates the economic extraction of metals from ores of lower a nd lower grades, whic h requires effi cient. skilled ben eficiation . Thus, careful study under the reflected-light mic roscope of the ore and ofthe products ofvarious co mminutio n and sepa ration processes is necessary. If, following initial disco very; exp lo ratory drilling to determi ne ove rall size,grade, a nd geo logical setting; mineralogical analysis to establish feasibili ty of metal extraction; and pilot testing of the extrac tion processes, it is decided to proceed with a mining operation, the ore micro sco pist is still needed to monitor variations in th e mineralogy of the ore and the effects ofsuch variations on processing.Variations laterally orvertically in the orebody ma y ca ll for cha nges in beneficia tion procedures or mixing of ores mined from different areas; the microscopi c study ofthe ores may also be of grea t value as a guide to mine exploration and development. In all ofthese applica tions, th e ore mineralo gy has to be related to th e geologica l and en gineering problems of mining, on the one hand, and to the problem s of beneficiation and metallurg ica l treatment, on th e othe r. REFERENCES 349 REFERENCES
Amstutz, G. C. (1961). Microscopy applied to mineral dressing. Colo. School Mines 56, 443-484. Basta, E. Z., EI Sharkowi, M. A , and Salem, M. W. (1969). Mineralogy ofsome fluxed sinters produced from the Aswan iron ore. Trans. /nst. Min. Metall. 78, CI-C13. Brock, M. (1993). "Microchemical Ch aracterization of Ash from Fuel Production." M.S. Thesis, Virginia Polytechnical Institute and State University, 1993,74 pp. Brooke, 1. N., and Prosser, A P. (1969). Manganese nodules as a source of copper and nickel-mineralogical assessment and extraction. Trans. /nst. Min. Metall. 78, CM cn Burn s, R G., and Burn s, V. M. (1977). Mineralogy. In G. P. Glasby (ed.), Marine Manganese Deposits, Elsevier Oceanography Series, No. IS. Elsevier, Amsterdam. _ _ . (1979). Manganese oxides. In Marine Minerals, Vo!. 6. Min . Soc. Am. Short Course Notes, pp. 1-46. Craig, 1. R, Ljokjell, P., and Vokes, F. M.(1984). Sph alerite compositional variation in sulfide ores of the Norwegian Caledonides. Econ. Geol. 79, 1727-1735. Cra ig, J. R., Najj ar, M. S., and Robin, A (1990). Characterization of coke gasification slags. In W. Petruk et a!. (eds.), Process Mineralogy /X The Metallurgical Society Warrendale. Pa.. pp. 473-483. Edwards ,A B. (1954).Texturesofthe OreMinerals and TheirSignijicance. Aust. Inst. Min . Metall., Melborne, Australia. Fletcher, A W. (1970). Metal winning from low grad e ore by bacterial leaching. Trans. Inst. Min. Metall. 79, C247-C252. Fuerstenau, D.W., and Han, K. N. (1977). Extractive metallurgy. In G. P. Glasby (ed.), MarineManganeseDeposits, Elsevier Oceanography Series, No. IS, Elsevier, Amster dam. Groen.J .C.(1992)."Microchemical phase characterization of petrol eum coke gasifica tion slags." Ph .D. Dissertation, Virginia Polytechnical Institute and State Univer sity, p. 132. Gaudin, A M. (1957). Flotation. McGraw-Hill, New York. Habashi, F. (1978). Chalcopyrite: Its Chemistry and Metallurgy. McGraw-Hill, New York. Hagni, R D. (1978). Ore microscopy applied to beneficiation. Min. Eng. 30, 11 37 1147. Jones, D. G.(1974). Optic al micros copy and electron-probe microanalysis study of ilmenite reduction. Trans. /nst. Min. Metall. 83, C I-C9. Jones, M. P. (1977).Automatic image an alysis. In J. Zussman (ed.),Physical Methods in Determinative Mineralogy. Academic, London, New York. Kirby,C. S., and Rim stidt.J, D.(1993).Mineralogy and surface properties of municipal solid waste ash. Environ. Sci. Technol. 27, 652-660. Mousoulos, L. and Papadopoulos, M. Z. (1976). Gravity concentration of Troodos chromites. Cyprus. Trans. /nst. Min. Metal/. 85, C73-C77. Petruk, W. (1990). Determining mineralogical characteristics by image analysis. In Advanced Microscopic Studies of Ore Minerals, J. L. Jambor and D.J. Vaughan (eds.), Mineral. Soc. ofCanada. Short course rates 17, Ottawa, pp. 409-425. 350 APPLICATIONS OF ORE MICROSCOPY IN MINERAL TECHNOLOGY
Pryor. E. J. (1965). Mineral Processing. Applied Science, London. Ramdohr, P. (1969). The are Minerals and Their Intergrowths. Pergam on, Oxford. Eng land. Reh wald, G. (1965). The application ofore microscopy in beneficiation ofores of the preciou s metals and ofthe nonferrous metal s. In H. Freund(ed.).Applied areMicros copy. Macmill an, New York. Schwartz. G. M.(1938). Reviewofthe app licat ion ofmicroscopic study to metallurgical pro blems. Econ. Geol. 33. 440-453. Willis. B. A. (1992).Mineral Processing Technology:An Introduction to the PracticalAspects of are Treatment of Mineral Recovery. 5th ed. Pergamon, Oxford.